Fractography andTensile Properties of AA6061AluminiumAlloy/ Rice Husk Ash Silicon Nanocomposite

'e unstoppable quest for low-cost reinforcing agent gingered the enthusiasm towards developing and utilising the agro-based waste product as reinforcement since they are promptly accessible, sustainable, and inexpensive to purchase. In this study, AA6061/rice husk ash matrix composites were produced through metallurgical stir casting techniques. Different weight percentages of reinforcement in the range of 2%, 4%, 6%, and 8% were used to fabricate the composites. 'e reinforced composites were characterized by SEM/EDS for microstructural study.'emechanical behaviour was examined for all the produced samples. SEM/EDS analysis revealed the presence of silica, a major constituent of rice husk ash in the produced composites. 'e results of the mechanical behaviour show that upgrading the weight percentage of reinforcing agent increases the mechanical properties. AA6061/8% rice hush ash generated a consistent rise with filler concentration in comparison with the aluminium alloy in all operating functions.


Introduction
e high cost of ceramic material prompts the use of ecofriendly inexpensive agro-based waste reinforcing materials on aluminium-based alloys for industrial application [1,2]. e utilization of modern technologies for reducing severe failures in major engineering component is necessary for metal construction industries as a result of its innovative qualities, and studies have revealed that aluminium alloy is the cheapest and global valuable materials [3,4]. Aluminium alloy is a class of aluminium with low density, light weight, ultimate tensile strength, and hardness [5,6].
e high demand for aluminium applied in the different application is unquantifiable to the implementation of other metals. Moreover, aluminium is utilized in numerous fields, starting from building construction to kitchen wares. Aluminium and its alloys are applied in numerous factories as a result of their encompassing properties such as higher strength-toweight ratios, decent corrosion resistance, and exceptional workability [7]. e production of aluminium is invariably broad as it embraces different stages of the metallurgical path. e quest to create cheaper materials, particularly metal matrix composites (MMCs) with enriched structures, has occupied the attention of many researchers [8,9]. Pure aluminium cannot be used for structural applications except when other elements are included in the substance to obtain sufficient strength for the production of structural members [10]. MMCs are utilized immensely in industrial processes involving light weight with stiffness, superspecific strength, ductility, and resistance due to heat [11]. Fly ash, fibres, whiskers, and particles are few examples of agro-based waste particulate used recently for reinforcement [12,13]. Numerous researchers desire to use cheaper materials to reinforce aluminium alloy, particularly metal matrix composite with superior properties [14]. However, AA6061 alloy has rough particles and enormous needle/plate-like eutectic silicon, which resulted in low mechanical behaviour. AA6061 alloys are a cluster of Al-Si-Mg and their rises in strength are by the processing of Mg 2 Si in the aluminium alloy [10]. e enthusiasm in the improvement of metal matrix composites (MMCs) is anchored on its mechanical applications for light materials with a unique quality, malleability, and thermal resistance [15]. e desire to produce inexpensive smart composite necessitates numerous inventions in the technological world. Among the several reinforcements used like silicon carbide and aluminium oxide, rice husk ash is the lowest reinforcement attainable in huge quantity as an agro-based waste [16,17]. Rice husk ash (RHA) was selected because of inherent composition such as silicon embedded in the material. Silicon has high melting and boiling points of 1414°C and 3265°C, which contributed to reducing the melting temperature of the produced composites.
In the current study, the use of AA6061/RHA composites to boost the structural properties of the material was determined. Senapati et al. explore the use of agro-based discarded RHA and fly ash to strengthen the aluminium alloy used in the manufacturing industry. e author deduced that the addition of fly ash and rice husk particulates in the aluminium alloy advances the matrix hardness and the wear properties of the composite [18]. Prasad and Krishna examined the mechanical features of AA356.2/RHA composites. e authors observed more anticipated surface morphology and mechanical characteristics than the as-received sample. e result depicts that the presence of RHA particles leads to the improvement in hardness and strength of the developed composite [2]. Subrahmanyam et al. carried out inoculation of aluminium alloy using agricultural waste rice husk ash. e authors observed that the mechanical properties of MMCs performed better with the inclusion of RHA in aluminium alloy. e microstructure with 8% RHA particles has exceptional mechanical properties and uniformly distributed particulates [19].
According to Haque et al., "the production of inexpensive metal matrix composites strengthened with ecofriendly material has contributed to revolutions in the field of engineering to limit environmental pollution". e authors fabricated and characterized the reinforcement of AA356.2 alloy with RHA particulates. e microstructure study reveals homogeneous dispersal of RHA particulates in the produced composites. Furthermore, it shows that the toughness measured by impact test increases as RHA content increases. It was affirmed that AA356.2/RHA composites could be utilized where light-weight materials are needed with better stiffness and strength [20].
Valyakala et al. studied the source of the destruction of a forced draft fan based on a study carried out in the petrochemical industry. e major factor affecting the failure rate of forced draft fan in a petrochemical industry was vibration, and vibration in turn caused bearing failure. e causes of failure of the fan blade are divided into four main parts: machine, material, equipment, and labour. e authors affirmed that suspended particles in the air instigate erosion on the blades. erefore, the authors concluded that forced draft fan damage was caused by bearing damage, and it can be evaded by eliminating disruption in the impeller and misalignment of base and fastener failure [21]. Kushwaha studied failure analysis and technique of averting fracture in the generator's fan blade. e authors concluded that the blade crack was due to fatigue situations in resonance state and the growth of existing small feasible cracks [22]. e research complications envisaged are the deformations of machine parts due to environmental generated failure altering the grain borderline.
e study provides agro-based waste to boost aluminium alloy in the manufacturing industries. e study aimed to determine the fractography and tensile properties of AA6061 aluminium alloy/rice husk ash silicon nanocomposite to curb the constant failure of equipment in the industry.

Matrix Material.
e matrix material used in this work is aluminium 6061. Aluminium 6061 is an alloy of aluminium whose main alloying elements are magnesium and silicon. is material is made use of in this work because of the mechanical properties it exhibits, such as strength and good welding ability. In the present study, the chemical composition of the matrix is shown in Table 1.

Reinforcement Materials.
In this study, the reinforcement material is rice husk ash. It is made from rice mill plant in Abakaliki, Ebonyi State. e RHA is cleaned with water to exclude the dust and dehydrated at room temperature for one day. Washed rice husk is then heated to 200°C for one hour to get rid of the moisture. It is then heated to 600°C for 12 h to eradicate the carbon content. e chemical element of RHA is shown in Table 2. Figure 1 shows the flowchart for the processing of rice husk ash.

Mechanical Properties.
Mechanical properties for prepared composites of varying reinforcements were assessed in hardness and tensile properties. e Brinell hardness was measured at a load of 100 g for 15 seconds. e universal testing machine (UTM) SM1000 was used in this work for testing the material tensile strengths.

Preparation of Composite Samples.
e production of AA6061/rice husk ash was done effectively by stir casting method. e study was carried out at different percentage compositions of reinforcement. Firstly, AA6061 is poured into the red heated electrical furnace and the temperature is raised to 750°C until total melting. Slag is extracted to generate good quality of the melt. e obtained RHA is preheated to 600°C in a detached oven and maintained for 20 minutes to eradicate moisture content. e picture of the stir cast arrangement is shown in Figure 2. e mechanical stirrer is dipped into the melt and slowly stirred to create a vortex. en the preheated rice husk ash is poured to the melt at a temperature of 720°C.
Concurrently, the stirring preparation is taken and transferred at a temperature of 650°C into the preheated moulds of 250 mm × 25 mm size cylindrical hole instantly. Precaution is ensured for the thorough conversion of the molten metal to solid. Figure 3 shows the developed composite material before the tensile test.

Hardness Testing.
e Brinell hardness experiment was done using a 10 mm steel ball indenter TQ SM1000 universal testing machine, the tiny circular specimens were placed in a cavity connected to the axis as a steel ball indenter, and then the steel ball using a lever having hydraulic energy is pushed into the sample for 10 s observation and continued reading the applied force on the digital readout screen. e diameter of the indentation on the samples was determined in a granule consisting of a magnifying glass having a weighing scale. e Brinell hardness value was based on the Brinell scale formula as follows: where HBS = H (hardness), B (Brinell), S (steel), F = applied force, D = diameter of indenter, and d = diameter of indentation [23].

Universal Material Testing
Machine. e SM1000 Universal Test Machine Cap 100 kN (10 ton) is used to determine the tensile strength of the developed composites. It is a universal test machine (UTM) commonly known as the universal tester. It is very versatile as it was used to perform the tensile strength tests. is is a multifunctional tensile and hardness testing machine.

Scanning Electron Microscope (SEM).
e scanning electron microscope (SEM) was used to perform the microstructural examinations and phase analysis for each reinforced sample. e microscope is reinforced by an energy dispersion spectrometer (EDS) to determine the quantified composite identity of the elements present in the working samples. For unified elementary research, the TESCAN scanning electron instrument enables high vacuum resolution separation. Figure 4 shows the SEM/EDS of as-received sample depicting the significant presence of aluminium from the EDS analysis. Figure 5 shows the microstructure of the developed composite prepared by stir casting methods. A homogeneous dispersal of RHA is noticed visibly in Figure 5(b) without cavities and gaps. Figure 6(b) shows the presence of eutectic silicon α-Al phase precipitation and uneven    International Journal of Chemical Engineering 3 distribution of particulate grain refiners. More developed and uniform dispersal of particulates is observed for the sample AA6061/8% RHA at 75 μm. It was noticed that a needle-like particle with well-structured crystal due to the improved arrangement of the reinforcement existed with the elemental composition of all basic collections seen at the EDS. It is interesting to note that the percentage of reinforcements plays a vital role in the stable modification of crystal. In this work, studies by Saravanan and Kumar stated that prospective ceramics particles have an intensity to cause consistent growth due to the nucleation system as seen in Figure 6(b) [24]. Siddharth and Rao stated that the addition of reinforcing agent led to the building of the silica-rich layer at the matrix margin [25].

Fractured Surface Analysis of AA6061/RHA Composite.
e fractured surfaces of the tensile specimens were examined using a scanning electron microscope (SEM), which gives the fracture propagation of the tensile specimens, and Figure 7 shows the fractured SEM image of the starting material. It revealed a flat fracture surface consisting of small fracture facets and tear ridges in the microstructure  International Journal of Chemical Engineering images of the starting material indicating that it is a ductile fracture. Figure 8(a) illustrates the detailed fracture surface morphologies of AA6061/2% RHA composites. e fractured SEM images show a flat fracture surface involving wear track and tear ridges. Maleque et al. stated that fracture occurs in composite material by crack initiation which followed immediately at the boundary between aluminium alloy and reinforcement, and the ductile properties are characterized by the wear track and tear ridges observed on the fractured surface [26]. Figure 8(b) shows the fractography of AA6061/4% RHA composites. It can be observed to have irregular tear ridges and less ductile failure due to more voids and fewer depths of dimple before reinforcements. Figure 8(c) shows the fractography analysis of AA6061/6% RHA composites. It revealed a noticeable dimple effect of the fracture surface, which specifies the ductility of the material. Figure 8(d) shows that AA6061/8% RHA has a higher tensile strength than the as-received sample because of the ductile nature of the material. However, AA6061/8% RHA reveals a noticeable fracture surface after tensile tests in macroscopic images and equal deep dimples spread over the fracture surface. Dimples enclose the greater area with considerable dimple depth and intermetallic segregation which is due to the reinforced agent present in the matrix [27,28]     RHA added to the matrix, the higher its tensile strength, thereby causing a boost in the mechanical properties [30]. Figure 11 shows the percentage elongation analysis and variable influence of the reinforced alloys for AA6061/RHA alloy in 75 μm grain sizes. From the compared process parameter, AA6061 + 8% RHA at 75 μm among the others gave a better superior percentage elongation than the asreceived sample. It is noticed that the elongation of composite reduced with the reduction in the percentage of the reinforcement [7].

Conclusion
e following conclusions were made: Agro-based waste rice husk ash particulate can be utilized for the production of MMCs for industrial applications. AA6061 was successfully reinforced with rice husk through a liquid metallurgy stir casting route. AA6061/8% RHA gives the maximum tensile value of 6339 kPa in comparison with the 6000 kPa for the asreceived sample in all operating conditions. e developed metal matrix agro-refiner alloy greatly improved the hardness from 152 BHN to 188 BHN at a performance influence of 23.7%.

Data Availability
e data used to support the findings of this study are included within the article.